Discussion Chain ID: 134191
================================================================================

User asked: How to identify if a material is perovskite or not?

This is more of a materials science question, but I believe many of you have referred [NIST Inorganic Crystal Structure Database (ICSD)](https://icsd.nist.gov/) database. I am collecting a database of perovskite materials and got a little bit confused on how the structure type is defined in the ICSD website. Please find a screen shot of ICSD results on lead zirconate titanate (PZT) material. [](https://i.sstatic.net/xCHBP.png) Here, when mole fraction $\ce{Zr}=0.52$, the 'Struct. Type' is defined as $\ce{FeNbPb2O6}$. Does it mean that PZT material when $\ce{Zr}=0.52$ is not perovskite? And in general if the column 'Struct. Type' does not start with 'Perovskite,' does that mean the material is not perovskite? Finally, sometimes I see the structure type named 'Elpasolie' or $\ce{LiNbO3}$ (disordered). Are these also perovskites? (or double perovskites?)

Answer 1 (3 votes):
As MaxW indicated in the comment, _perovskites_ are a huge family of natural and synthetic compounds. Following is a breif description of the group of compounds named _perovskites_ : The original Perovskite is a mineral of formula $\ce{CaTiO3}$. It was first discovered in 1839 by the Prussian minaralogist Gustav Rose in the Ural Mountains, and is named after Russian mineralogist Count Lev Aleksevich von Perovski (1792–1856). The natural crystals have a hardness of 5.5-6 and a density of $\pu{4000-4300 kgm-3}$. The crystal structure of this mineral was initially thought to be cubic, but was later shown to be orthorhombic (Ref.1). As with many minerals, Perovskite has given its name to a family of compounds with the same type of crystal structure, which are called _perovskites_ that have a general formula close to or derived from the composition $\ce{ABX3}$. In these mineral type with formula $\ce{ABX3}$, $\ce{A}$ and $\ce{B}$ are usually two different sized cations, while $\ce{X}$ is an anion that bonds to both (_e.g._ , $\ce{KNbO3}$). For instance, $\ce{PbTiO3}$) is a _perovskite_ , crystals of which are Tetragonal (space group: $P_4mm$) with $a=\pu{0.3902 nm}$ and $c=\pu{0.4143 nm}$ of its unit cell. In contrast, the original Perovskite, $\ce{CaTiO3}$ crystals are Orthorhombic (space group: $Pbmn$) with $a=\pu{0.54035 nm}$, $b=\pu{0.54878 nm}$ and $c=\pu{0.76626 nm}$ of its unit cell (Ref.1). To some extent, the multiplicities of phases that belong to the _perovskites_ family can be rationalized by assuming that _perovskites_ are simple ionic compounds where $\ce{A}$ is usually a large cation and $\ce{B}$ is usually a medium-sized cations, and $\ce{X}$ is an anion (if the charges of the ions are written as $q_\ce{A}$, $q_\ce{B}$, $q_\ce{X}$, then: $q_\ce{A} + q_\ce{B} = 3q_\ce{X}$). At present, many hundreds of compounds are known that adapt the _perovskite_ structure. Few examples are $\ce{NaMgF3}$ (Orthorhombic; space group: $Pbnm$), $\ce{CsPbI3}$ (Cubic; space group: $Pm \overline{3} m$), $\ce{KCuF3}$ (Tetragonal; space group: $I4/mcm$), $\ce{LaAlO3}$ (Trigonal; space group: $R3c$), $\ce{KNbO3}$, $\ce{KNbO3}$ (Orthorhombic; space group: $Amm2$), and $\ce{(Fe,Mg)SiO3}$ (Orthorhombic; space group: $Pnma$). In fact, a _perovskite_ structure mineral, _Bridgmanite_ $\left(\ce{(Fe,Mg)SiO3}\right)$ is the most abundant solid phase in the Earth’s interior, making up $38\%$ of the total (Ref.1). Figure **A** in following diagram illustrates an ideal cubic _perovskite_ , $\ce{SrTiO3}$ (space group: $Pm \overline{3} m$): [](https://i.sstatic.net/ne2mQ.jpg) The traditional view of the _perovskite_ lattice is that it consists of smaller $\ce{B}$ cations within oxygen octahedra, and larger $\ce{A}$ cations which are nine fold coordinated by oxygen. According to [this Princeton website](https://www.princeton.edu/~cavalab/tutorials/public/structures/perovskites.html) where I abstracted the structure **A** (**Note:** I have modified to some extent): > The easiest way to visualize the structure ($\ce{ABO3}$) is in terms of the $\ce{BO6}$ octahedra (_e.g._ , $\ce{TiO6}$), which share corners infinitely in all 3 dimensions, making for a very nice and symmetric structure. The $\ce{A}$ cations ($\ce{Sr}$) occupy every hole which is created by 8 $\ce{BO6}$ octahedra, giving the $\ce{A}$ cation a 12-fold oxygen coordination, and the $\ce{B}$-cation a 6-fold oxygen coordination. In the example shown below, ($\ce{SrTiO3}$) the $\ce{Sr}$ atoms sit in the 12 coordinate $\ce{A}$ site, while the $\ce{Ti}$ atoms occupy the 6 coordinate $\ce{B}$ site. Note that there are many $\ce{ABO3}$ compounds for which the ideal cubic structure is distorted to a lower symmetry (_e.g._ , tetragonal, orthorhombic, etc.). Based on these facts, your last two entries, $\ce{Pb(Zr_{0.45}Ti_{0.55})O3}$ and $\ce{Pb(Zr_{0.871}Ti_{0.129})O3}$, are of course belong to _perovskite_ family. The first one have adapted to the structure of $\ce{PbTiO3}$ (Tetragonal; space group: $P_4mm$), which is a _perovskite_ (Ref.1). The second one have adapted to the structure of $\ce{LiNbO3}$ (Trigonal; space group: $R3c$), which is a synthetic _perovskite_ ([Wikipedia](https://en.wikipedia.org/wiki/Lithium_niobate)). There is another family of compounds with formula $\ce{A2BB'O6}$, which is called _double perovskites_. The crystal structures of _double perovskites_ feature an ordered rock-salt like arrangement of corner-sharing $\ce{BO6}$ and $\ce{B'O6}$ units in the crystal structure (Figure **B**). This is what researchers in [Max Plank Institute](https://www.cpfs.mpg.de/2486283/Double-perovskites) where I have extracted the Figure **B** have to say about _double perovskites_ : > Proper choice of the metal ions $\ce{B}$ and $\ce{B'}$ and of the alkali, alkaline earth, or rare earth ions $\ce{A}$ allows to realize a large variety of physical properties in _double perovskites_. Prototype compounds which have found much interest are $\ce{Sr2FeMoO6}$ and $\ce{Sr2FeReO6}$ as they are half-metallic ferromagnets with Curie temperatures above room temperature and large magnetoresistance effects at ambient conditions. The _double perovskite_ structure is so named because the unit cell of _double perovskite_ is twice that of usual _perovskite_. An example of crystal structure of a synthetic _double perovskite_ , $\ce{Sr2FeMoO6}$, is shown in Figure **C** , which has a Orthorhombic (Phase Prototype: $\ce{Sr2WNiO6}$; space group: $Cmme$) unit cell (Ref.2). It has the same architecture of 12 coordinate $\ce{A}$ sites and 6 coordinate $\ce{B}$ sites, but two cations are ordered on the $\ce{B}$ site. The structure of $\ce{Sr2FeMoO6}$ shown here,the $\ce{Fe}$ and $\ce{Mo}$ atoms have ordered in a 3D chessboard type fashion. Hence, it is safe to suggest that the compound used for first three entries, $\ce{Pb(Zr_{0.52}Ti_{0.48})O3}$, is an example of _double perovskites_ , solely because it has a prototype structure of $\ce{Pb2FeNbO6}$ (Monoclinic; space group: $Cm$), which resembles a _double perovskite_ ($\ce{A2BB'O6}$ type). The crystal structure of $\ce{PbFe_{0.5}Nb_{0.5}O3}$ is slightly distorted cubic ($a = b = c = \pu{4.0056 \mathring A}$; and $\alpha = \beta = \gamma = \pu{89.664 ^\circ C}$) and declaired to be a _perovskite_ (Ref.3). On the hind site, $\ce{PbFe_{0.5}Nb_{0.5}O3}$ resembles more of $\ce{Pb(Zr_{0.52}Ti_{0.48})O3}$ than that of $\ce{Pb2FeNbO6}$. * * * **Note:** The best advice to OP is start with the book (Ref.1), which is written in basic language, understandable for any novice student learning about Perovskite materials. In addition, since OP is conveniently in England, I believe he can consult the author of the book, Prof. Richard J. D. Tilley, Ph.D., the Emeritus Professor in the School of Engineering at the University of Cardiff, Wales, United Kingdom, if OP has additional questions on Perovskite materials. * * * **References:** 1. Richard J. D. Tilley, In _Perovskites: Structure-Property Relationships_ ; John Wiley & Sons Ltd.: Chichester, West Sussex, United Kingdom, 2016 (ISBN: 978-1-118-93566-8). 2. Y. C. Hu, J. J. Ge, Q. Ji, B. Lv, X. S. Wu, G. F. Cheng, "Synthesis and crystal structure of double-perovskite compound $\ce{Sr2FeMoO6}$," _Powder Diffraction_ **2010** , _25(S1)_ , S17-S21 (<https://doi.org/10.1154/1.3478711>). 3. Renbing Sun, Wei Tan, Bijun Fang, "Perovskite phase formation and electrical properties of $\ce{Pb(Fe_{1/2}Nb_{1/2})O3}$ ferroelectric ceramicse," _Physica Status Solidi A: Applications and Meterial Science_ **2009** , _206(2)_ , 326-331 (<https://doi.org/10.1002/pssa.200824432>).

Discussion on this answer:
Comment: Excellent! This is a perfectly compiled answer that is so rich in information and I can't thank you enough for it. I believe I must do more research on perovskite materials, however, there seems to be a bit of controversy among scientists too, for defining a decision boundary between perovskites and non-perovskites. For an example, LiNbO3 may be identified as a synthetic perovskite, however, some [studies](https://pubmed.ncbi.nlm.nih.gov/21604713/) differentiate between perovskite and LiNbO3 structures. Finally, if you think the question shadows this great answer, please edit the question.
Comment: @ Achintha: No need to change anything. That's why I put the infor of auther who lives in UK, so he can contribute (I assume it'd be similar in UK, alike here in US! :-) Good luck.

Answer 2 (1 votes):
The HMS column is for the **H** ermann–**M** auguin **S** ymbol. You can see the line for 55700 has "P4mm" which is the proper crystal symmetry to be of the Perovskite structure. That line is also notated "Perovskite#PbTiO3#B". So of the formulations listed that is the only one that has the Perovskite crystal structure.

Discussion on this answer:
Comment: Sorry to ask this question again as it might be opinion based. But I found [elsewhere](https://books.google.co.uk/books?id=o0pJnnQRq-UC&pg;=PA22&lpg;=PA22&dq;=pb2fenbo6+perovskite&source;=bl&ots;=cCCfPCMtte&sig;=ACfU3U3xgRl5umusoIdCzuE8l70fZh38bg&hl;=en&sa;=X&ved;=2ahUKEwjP06ut4crpAhVoRhUIHaUeDXoQ6AEwAHoECAQQAQ#v=onepage&q;=pb2fenbo6%20perovskite&f;=false) that Pb2FeNbO6 is perovskite. Doesn't is make the first 3 materials in the image perovskite too?
Comment: Perovskite itself is the mineral $\ce{CaTiO3}$. Exactly how the huge family of the synthetic perovskite derivatives fits together I do not know.


================================================================================

